Advances in Materials Physics and Chemistry, 2013, 3, 19-30 http://dx.doi.org/10.4236/ampc.2013.31A003 Published Online April 2013 (http://www.scirp.org/journal/ampc)
Small-Angle X-Ray Scattering of Amorphous Germanium: Numerical Modeling
R. Ben Brahim, A. Chehaidar* Research Unit in Mathematical Physics, Department of Physics, Faculty of Sciences, University of Sfax, Sfax, Tunisia
Email: *[email protected]
Received January 13, 2013; revised February 27, 2013; accepted April 4, 2013
Copyright © 2013 R. Ben Brahim, A. Chehaidar. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
ABSTRACT The present work deals with a detailed analysis of the small-angle X-ray scattering of nanoporous atomistic models for amorphous germanium. Structures with spherical nanovoids, others with arbitrarily oriented ellipsoidal ones, with monodisperse and polydisperse size distributions, were first generated. After relaxing the as-generated structure, we compute its radial distribution function, and then we deduce by the Fourier transform technique its X-ray scattering pattern. Using a smoothing procedure, the computed small-angle X-ray scattering patterns are corrected for the termina- tion errors due to the finite size of the model, allowing so, for the first time at our best knowledge, a rigorous quantita- tive analysis of this scattering. The Guinier’s law is found to be valid irrespective of size and shape of the nanovoids over a scattering vector-range extending beyond the expected limit. A weighted combination of the Guinier’s forms accounts for well the nanovoid size distribution in the amorphous structure. The invariance of the Q-factor and its relationship to the void volume fraction are also confirmed. Our findings support then the quantitative analyses of available small-angle X-ray scattering data for amorphous germanium. Keywords: Amorphous Germanium; Structure; Small-Angle X-Ray Scattering; Modeling
1. Introduction Amorphous semiconductors have been the subject of ex- tensive experimental and theoretical investigations. Most of the interest has been focused on the tetrahedrally-co- ordinated amorphous germanium (a-Ge) due to its simple chemical bonding and composition on the one hand, and its potential applications in the fields of microelectronics and energy-conversion technologies on the other hand. As with all materials, the microstructure controls the electrical as well as the optical properties, so understand- ing and controlling the structure of a-Ge is crucial to its technological applications.
Unlike the crystalline phase, there is no experimental technique available that can determine the coordinates of atoms in a-Ge. Direct experimental data about atomic structure in amorphous materials were essentially limited to structure factors derived from X-ray, electrons, or neu- tron diffraction experiments . Conventional diffraction measurements, principally, show that a-Ge, and other materials that form covalent tetrahedrally bonded crystals maintain the same pattern of four nearest neighbors in the
amorphous phase, but do not have the long-range transla- tional order that leads to sharp diffraction peaks. Small- angle scattering experiments performed on some a-Si and a-Ge films have shown a rapid increase of the scattered intensity as the scattering vector goes to zero [2-11]. More- over, the shape and the magnitude of this small-angle scattering are found to be strongly dependent on the growth conditions and change after processing steps such as annealing or light illumination [12,13]. It is well known that such feature in the small-angle scattering data mirrors the heterogeneity of the amorphous material at the nanoscale. By correlating small-angle scattering re- sults with those derived from other experiments [14-20], the mass-density measurements principally , many authors have postulated the existence of nanovoids in a-Si and a-Ge films. Indeed, such structural inhomoge- neities are commonly believed to result in the mass-den- sity of a-Si and a-Ge being lower than their correspond- ing crystalline phases; they also generate significant fluc- tuations in the density at the nanoscale which can be at the origin of the intense small-angle scattering in these materials. Many attempts have been made to analyze quantitatively the small-angle scattering data in a-Si and *Corresponding author.
Copyright © 2013 SciRes. AMPC
R. B. BRAHIM, A. CHEHAIDAR 20
a-Ge. Using theoretical laws established previously , some characteristics of the nanovoids in these amorphous materials, such as size distribution, shape and number density, have been deduced from small-angle scattering data.
Numerical modeling technique has been widely used to simulate the structure of a-Ge. Most of the effort has been devoted to the analysis of its homogeneous struc- ture; the generally accepted topological model is the so- called continuous random network (CRN). In this model, the main building blocks of the material are the same as in its crystalline counterpart, i.e. tetrahedra of Ge, but unlike in a perfect crystal, these blocks can be randomly oriented and connected, allowing “play” in atomic bond- lengths and angles. Several approaches have been pro- posed for representing a homogenous tetrahedrally coor- dinated CRN models (see [22-24] and references therein). Most of these networks successfully reproduce the so- called wide-angle scattering data, i.e. for scattering vec- tors upper than 1 Å−1. Some numerical simulations deal- ing with nanovoids in a-Si have been also reported in the literature [25-31], but only two, to the best of our know- ledge, are interested in the small-angle scattering [25,26]. Biswas et al.  were the first to demonstrate that CRN in which nanovoids are created accounts for the intense small-angle scattering, without altering the wide-angle scattering pattern. In our previous work , we have shown that CRN model containing nanocrystallites, called paracrystalline model , does not realize the intense small-angle scattering; paracrystalline networks contain- ing nanovoids, on the other hand, account for the mass- density deficit and also the small-angle scattering feature observed experimentally. Due to computational limita- tions, unfortunately, relatively small atomistic models have been examined. However, it is well known that the small-angle scattering pattern is very sensitive to the model size. Indeed, the finite size of the structure im- poses a scattering-vector threshold ( 2π L
≈ , where L is the size of the model), a features broadening, and also results in spurious ripples in the scattered intensity. In- creasing the size of the atomistic model allows pushing down the scattering-vector threshold and reduces the amplitude of the ripples. Recently, Graff and Thorpe  have used a very large CRN model (105 atoms) to simu- late the long-wavelength limit of the structure factor of amorphous silicon. Despite this huge model size, how- ever, the scattering-vector threshold has moved very little (0.05 Å−1 vs 0.1 Å−1 for 4096-atom model), and the most remarkable is the persistence of the small-angle spurious ripples in the structure factor. The question that arises is then: how to make a good estimate of the scattered inten- sity free of finite model-size effects?
In the present work we reexamine the structural prop- erties of atomistic models for a-Ge with nanovoids. We
pay particular attention to the X-ray small-angle scatter- ing. We consider structural models larger and more real- istic than those considered in our previous work. We propose a simple way to get rid of finite model-size ef- fects. A quantitative analysis of the estimated small-an- gle X-ray scattering is performed and comparison with available experimental data is made.
2. Computation Method The present investigations are based on the class of CRN models generated with the Wooten-Winer-Weaire bond- switching algorithm by Barkema and Mousseau , resulting in N-atom models with periodic boundary con- ditions. 4096-atom models are provided to us by the courtesy of Normand Mousseau. To generate voids in the preceding amorphous network, a cluster of atoms is re- moved within a prescribed volume centered on a site selected at random. By choosing the centers of the voids to be sufficiently far apart, a number of non-overlapping voids are then constructed. After this, the dangling bonds, thus created on the void surface, are rebonded; in prac- tice, the reconstruction of dangling bonds that would produce an unrelaxed bond of length greater than the second-neighbor distance (4 Å) and four-membered rings is rejected.
In order to obtain the equilibrium coordinates of these structures, a relaxation procedure is needed to minimize the deformation energy of the system. In the present work, the anharmonic Keating model proposed by Rücker and Methfessel  was used. Within the framework of this model, the strain energy of the system is given by:
( )222 20 0 , , ,
1 3ij ij ij ijk ij iki j i j k
V r rα β= − + +⋅ ⋅ r r r r
The first sum in this expression is on all atoms i in the supercell and their nearest-neighbors specified by j. The second sum is on all atoms i and pairs of distinct neighbors. ij and ik are the vectors connecting atom i with it
Click here to load reader